# G1RT-CT D. EXAMPLES F. GUTIÉRREZ-SOLANA S. CICERO J.A. ALVAREZ R. LACALLE W P 6: TRAINING & EDUCATION

Save this PDF as:

Size: px
Start display at page:

Download "G1RT-CT-2001-05071 D. EXAMPLES F. GUTIÉRREZ-SOLANA S. CICERO J.A. ALVAREZ R. LACALLE W P 6: TRAINING & EDUCATION"

## Transcription

1 D. EXAMPLES 316

2 WORKED EXAMPLE I Infinite Plate under fatigue Introduction and Objectives Data Analysis 317

3 INTRODUCTION AND OBJECTIVES One structural component of big dimensions is subjected to variable loading conditions everyday: 200 MPa during 12 hours and 20 MPa the rest of the day. During the maximum loading conditions other variable stresses appear, with a variation of 30 MPa (because of vibrations with a frequency 50 Hz). Some NDT are performed, with equipment whose sensitivity is 0.2 mm and no cracks are detected. Considering the component as an infinite plate: a) Determine the crack length which is necessary to crack propagation because of vibrations b) Critical crack length for final failure c) Life time for the component d) Evolution of the crack length with time in order to determine inspection periods 318

4 DATA Material properties: K IC = 100 MPa m 1/2 ΔK th (or ΔK 0 ) = 3 MPa m 1/2 if R = P min /P max = 0.1 ΔK th = 1.5 MPa m 1/2 if R = P min /P max = 0.85 Paris Law: da dn = (ΔK) 2 da/dn in m/cycle when ΔK in MPa m 1/2 319

5 Working conditions are plotted in the next figure: σ ( M P a ) h 2 4 h t ( h ) 320

6 The component geometry can be simplified as: σ 2a 2W The equipment sensitivity is 0.2 mm and no crack has been detected. So, in the worst possible situation 2a = 0.2 mm. 321

7 State I: VIBRATIONS σ ( M P a ) h 2 4 h t ( h ) R = P max /P min = 0.8 ΔK th = 1.5 MPa m 1/2 ΔK = Δσ (π a) 1/2 = 30 (π ) 1/2 = 0.53 MPa m 1/2 < ΔK th Existing cracks don t propagate 322

8 State II: MAIN LOADING CONDITIONS σ ( M P a ) h 2 4 h t ( h ) As R = 0.10 ΔK th = 3.0 MPa m 1/2 ΔK = Δσ (π a) 1/2 = 180 (π ) 1/2 = 3.19 MPa m 1/2 > ΔK th Existing cracks could propagate 323

9 As existing cracks could propagate, it is necessary to determine the crack length for crack propagation because of vibrations: ΔK th = 1.5MPa m 1/2 = 30 π a v a v = 0.80 mm For shorter cracks propagation is only due to main loading variation (Δσ =180 MPa, f = 1/86400 Hz) The critical crack length determined at failure is: K a f I max = σ max = 68 mm π a c = 215 π a f = 100MPa m For crack length over 0.80 mm propagation is due to both main loading variation and vibrations (Δσ = 30 MPa, f = 5 Hz) 1/2 324

10 LIFE TIME: The time necessary to initiate the effects of vibrations to cause crack propagation is determined through the Paris law: 1 a f N = Ln = Ln = 2042 cycles C Y ( Δσ) π a 1 10 (180) π cycles is equivalent to 2042 days or 5.59 years Once this crack length is reached, propagation is due to vibrations (mainly): a 0 = 0.8 mm a f = 68 mm 1 a f 1 68 N = Ln = Ln C Y ( Δσ) π a (30) π cycles is equivalent to 0.73 days 2 = cycles The same day that cracks achive length to propagate due to vibration amplitude, the component fails. SO, LIFE TIME IS 5.59 YEARS. 325

11 The evolution of semicrack length with time is (question d)): a ( m m ) 6 8 It is reasonable to define periodical inspections to check if really cracks propagate over the detectable value of 0.2 mm in total length (i.e. every two years) inspection in 2 years. cracks detected? No 0, 8 0, 1 5,59 ye a r s Yes Evaluate remanent life and take decisions 326

12 WORKED EXAMPLE II Fatigue test Introduction and data Objectives Analysis 327

13 INTRODUCTION AND DATA A fatigue test on a seven wire strand was performed. The maximum applied stress is 0.8 σ u and the amplitude is 390 MPa. The strand is one meter long and the diameter of the wires is 5 mm. The test finished with three broken wires, the central one and two external (which were together), after fatigue cycles (f = 8 Hz). The SEM observation of the failure surfaces gave the following information about crack lengths: - Central wire: 0.25 mm (depth) elliptical crack from non propagated initial defect. - External wire A: 1.32 mm from a non differentiated initial defect. - External wire B: 1.20 mm proceeding from a 0.30 mm in depth initial defect. From a previous tension test, the mechanical behaviour of the strand was obtained: E = 195 GPa Failure Load = kn Strain for Failure Load = 4.7 % (gauge base 500 mm) 328

14 OBJECTIVES From the testing results and the behaviour of the material, determine: a) The failure sequence of the wires as well as their form of failure and the fracture toughness of the material. b) Fatigue behaviour of the material considering a Paris exponent of 2.4 and the depth of the initial defect of wire A. a Consider for the wire geometry that K I = 2.12 σ a

15 The area of each wire is: A w = π r 2 = π = mm 2 Therefore, the area of the strand is A = 7 A w = = mm 2 The failure load is kn, so the failure stress can be calculated: σ f = / =1864 MPa The maximum and minimum stresses are: σ max = 0.8 σ f = = MPa σ min = 0.8 σ f 390 = = MPa 330

16 Under these conditions, the first failure occurs in the external wire A because it has the bigger propagated defect. After that, the external wire B breaks and finally, the central one. The external wire A breaks because of a fracture failure as a consequence of a fatigue process. Then: K I = 2.12 σ a c 0.5 = ( ) 0.5 = MPa m 1/2 K IC = MPa m ½ 331

17 The external wire B also fails because of fracture, but with a smaller defect because the decrease of the section once the external wire A is broken. The new supported σ max is: σ max = 7/ = MPa This stress is smaller than the failure strength of the strand (1864 MPa). Therefore, failure happens as a consequence of sudden fracture or plastic collapse. This later as the applied stress ( MPa) is close to yield stress (even non considering a possible strain hardening effect, then σ ymax = σ u = 1864 MPa) 332

18 We can calculate the stress intensity factor: K I = 2.12 σ a c 0.5 = (0.0012) 0.5 K I = MPa m ½ This value is bigger than K IC and it justifies the sudden failure of the external wire B. Now, there are only five wires in the section of the strand, so: σ max = 6/ = MPa This stress is bigger than the failure stress of the cord (1864 MPa). Therefore, it is possible to affirm that the latest is the maximum stress in the strand, and the central wire fails because of tension. In effect, the necessary stress for fracture to occur would be: = 2.12 σ σ = 3428 MPa Such a value is not reached at any time. 333

19 Let s now determine the fatigue properties of the material. We know that the central wire had a defect of 0.25 mm which did not produce crack propagation under Δσ = 390 MPa. So: ΔK th > 2.12 Δσ a 0.5 = = MPa m 1/2 We also know that an initial defect of 0.3 mm propagates in the external wire B and that the unknown initial defect of wire A should be higher than 0.3 because it reached a bigger final crack. So: ΔK th < 2.12 Δσ a 0.5 = = MPa m 1/2 From both expressions the threshold SIF is limited from the following values: < ΔK th < MPa m 1/2 334

20 The Paris law is: da dn 2.4 = C ( ΔK) = C (2.12 Δσ a ) 2.4 where C has to be defined We know: Δσ = 390 MPa So: da dn = C ( 2.4 ΔK ) = C ( a ) a i a f = da 2. C ( ) 4 dn 1.2 a = a = 0.3 mm C N a i f = 1.2 mm N = cycles conditions at wire B 335

21 C = = Therefore, the Paris law is: da dn = ( ΔK) 2.4 To calculate the initial defect in the external wire A, we will integrate the Paris law: 12 C = a 0.2 i a f = C N a f = 1.32 mm N = cycles a i = C N = a i = mm 336

### MAE 20 Winter 2011 Assignment 6

MAE 0 Winter 011 Assignment 6 8.3 If the specific surface energy for soda-lime glass is 0.30 J/m, using data contained in Table 1.5, compute the critical stress required for the propagation of a surface

### C. PROCEDURE APPLICATION (FITNET)

C. PROCEDURE APPLICATION () 495 INTRODUCTION ASSESSMENT OF SCC ASSESSMENT OF CORROSION FATIGUE STRESS CORROSION AND CORROSION FATIGUE ANALYSIS ASSESSMENT OF LOCAL THINNED AREAS 496 INTRODUCTION INTRODUCTION

### FAILURE MODES and MATERIALS PROPERTIES. Component failures. Ductile and Brittle Fracture COMPONENT FAILURES. COMPONENT FAILURE MODES examples:

FAILURE MODES and MATERIALS PROPERTIES MECH2300 - Materials Lecture 10 R. W. Truss Materials Engineering R.Truss@uq.edu.au COMPONENT FAILURES Structures lectures es on component es cause response in component

### Principles of Fracture Mechanics

8-1 CHAPTER 8 FAILURE PROBLEM SOLUTIONS Principles of Fracture Mechanics 8.1 This problem asks that we compute the magnitude of the maximum stress that exists at the tip of an internal crack. Equation

### Fatigue Testing. Objectives

Laboratory 8 Fatigue Testing Objectives Students are required to understand principle of fatigue testing as well as practice how to operate the fatigue testing machine in a reverse loading manner. Students

### Fatigue crack propagation

1 (20) Repetition Ð Crack initiation and growth Small cracks Shear driven Interact with microstructure Mostly analyzed by continuum mechanics approaches Large cracks Tension driven Fairly insensitive to

### Griffith theory of brittle fracture:

Griffith theory of brittle fracture: Observed fracture strength is always lower than theoretical cohesive strength. Griffith explained that the discrepancy is due to the inherent defects in brittle materials

### ME 215 Engineering Materials I

ME 215 Engineering Materials I Chapter 3 Properties in Tension and Compression (Part III) Mechanical Engineering University of Gaziantep Dr. A. Tolga Bozdana www.gantep.edu.tr/~bozdana True Stress and

### 9. TIME DEPENDENT BEHAVIOUR: CYCLIC FATIGUE

9. TIME DEPENDENT BEHAVIOUR: CYCLIC FATIGUE A machine part or structure will, if improperly designed and subjected to a repeated reversal or removal of an applied load, fail at a stress much lower than

### σ m using Equation 8.1 given that σ

8. Etimate the theoretical fracture trength of a brittle material if it i known that fracture occur by the propagation of an elliptically haped urface crack of length 0.8 mm and having a tip radiu of curvature

### B. INTRODUCTION TO ASSESSMENT PROCEDURES FOR CRACKED COMPONENTS

B. INTRODUCTION TO ASSESSMENT PROCEDURES FOR CRACKED COMPONENTS 40 INTRODUCTION HOW ARE INTEGRITY, SECURITY OR CRITICAL CONDITIONS ANALYSED IN A CRACKED STRUCTURE? FRACTURE MECHANICS Critical conditions

### CHAPTER 4 TENSILE TESTING

CHAPTER 4 TENSILE TESTING EXERCISE 28, Page 7 1. What is a tensile test? Make a sketch of a typical load/extension graph for a mild steel specimen to the point of fracture and mark on the sketch the following:

### Damage due to fatigue occurs when loading is markedly varying in time. R decreases with time S T. MSÚ F max

5. Fatigue of steel structures Fatigue loading, Wöhler s approach and fracture mechanics, fatigue strength, influence of notches, damage accumulation, Eurocode approach. Damage due to fatigue occurs when

### MAE 20 Winter 2011 Assignment 5

MAE 20 Winter 2011 Assignment 5 6.7 For a bronze alloy, the stress at which plastic deformation begins is 275 MPa (40,000 psi), and the modulus of elasticity is 115 GPa (16.7 10 6 psi). (a) What is the

### ME111 Lecture 16 1. ME111 Instructor: Peter Pinsky Class #16 November 1, 2000

Toda s Topics ME111 Instructor: Peter Pinsk Class #16 November 1, 2000 Introduction to linear elastic fracture mechanics (LEFM). Problem 3 A center-cracked plate of AII 1144 steel ( C = 115MPa m ) has

### G1RT-CT-2001-05071 A. BASIC CONCEPTS F. GUTIÉRREZ-SOLANA S. CICERO J.A. ALVAREZ R. LACALLE W P 6: TRAINING & EDUCATION

A. BASIC CONCEPTS 472 PROCESSES LOADING RATE Static or Quasi-Sstatic Dynamic MATERIAL ENVIRONMENT Liquid or Gaseous Environments AGGRESSIVE ENVIRONMENT MECHANIC LOADS Stress corrosion cracking (SCC) Corrosion

### STRAIN-LIFE (e -N) APPROACH

CYCLIC DEFORMATION & STRAIN-LIFE (e -N) APPROACH MONOTONIC TENSION TEST AND STRESS-STRAIN BEHAVIOR STRAIN-CONTROLLED TEST METHODS CYCLIC DEFORMATION AND STRESS-STRAIN BEHAVIOR STRAIN-BASED APPROACH TO

### Cracking Of Carbon Steel Components Due To Repeated Thermal Shock

Cracking Of Carbon Steel Components Due To Repeated Thermal Shock J W H Price, M Chang and B Kerezsi Department of Mechanical Engineering, Monash University, PO Box 197, Caulfield East, VIC 3145, Australia

### Mechanical Metallurgy

Mechanical Metallurgy Lecturer Assessment Dr. Assignment 20 (homework, quiz, attendance) Midterm exam 40 Final exam 40 Total 100 Mechanical Metallurgy Subject of interests Part I Mechanical fundamentals

### CH 6: Fatigue Failure Resulting from Variable Loading

CH 6: Fatigue Failure Resulting from Variable Loading Some machine elements are subjected to static loads and for such elements static failure theories are used to predict failure (yielding or fracture).

### ME311 Machine Design

ME Machine Design Lecture 5: Fully-Reversing Fatigue and the S-N Diagram W Dornfeld Oct26 Fairfield University School of Engineering Discovering Fatigue With the Industrial Revolution came the steam engine

### ANALYSIS OF THE FATIGUE STRENGTH UNDER TWO LOAD LEVELS OF A STAINLESS STEEL BASED ON ENERGY DISSIPATION

EPJ Web of Conferences 6, 6 38009 (00) DOI:0.05/epjconf/000638009 Owned by the authors, published by EDP Sciences, 00 ANALYSIS OF THE FATIGUE STRENGTH UNDER TWO LOAD LEVELS OF A STAINLESS STEEL BASED ON

### Assessment of Fatigue Cracks in Rails

Procedia - Social and Behavioral Sciences 00 (2011) 000 000 Procedia Social and Behavioral Sciences www.elsevier.com/locate/procedia Conference Title (Transport Research Arena Europe 2012) Assessment of

### IMPELLER FATIGUE ASSESSMENT USING AN S-N APPROACH

ENGINEERING PAPER 5244-08 IMPELLER FATIGUE ASSESSMENT USING AN S-N APPROACH Samuel Orr Engineering Analysis Manager Howden Technology AMCA International Engineering Conference Las Vegas, NV, USA 2 4 March

### Objective To conduct Charpy V-notch impact test and determine the ductile-brittle transition temperature of steels.

IMPACT TESTING Objective To conduct Charpy V-notch impact test and determine the ductile-brittle transition temperature of steels. Equipment Coolants Standard Charpy V-Notched Test specimens Impact tester

### NOTCHES AND THEIR EFFECTS. Ali Fatemi - University of Toledo All Rights Reserved Chapter 7 Notches and Their Effects 1

NOTCHES AND THEIR EFFECTS Ali Fatemi - University of Toledo All Rights Reserved Chapter 7 Notches and Their Effects 1 CHAPTER OUTLINE Background Stress/Strain Concentrations S-N Approach for Notched Members

### Accelerated Corrosion Fatigue Studies on SA 333 Gr.6 Carbon Steel

Accelerated Corrosion Fatigue Studies on SA 333 Gr.6 Carbon Steel P. S. Aarthi 1, G. Raghava 2, S. Vishnuvardhan 3, M. Surendar 4 P.G. Student, Department of Civil Engineering, Easwari Engineering College,

### ( ) = ( ) = {,,, } β ( ), < 1 ( ) + ( ) = ( ) + ( )

{ } ( ) = ( ) = {,,, } ( ) β ( ), < 1 ( ) + ( ) = ( ) + ( ) max, ( ) [ ( )] + ( ) [ ( )], [ ( )] [ ( )] = =, ( ) = ( ) = 0 ( ) = ( ) ( ) ( ) =, ( ), ( ) =, ( ), ( ). ln ( ) = ln ( ). + 1 ( ) = ( ) Ω[ (

### different levels, also called repeated, alternating, or fluctuating stresses.

Fatigue and Dynamic Loading 1 Fti Fatigue fil failure: 2 Static ti conditions : loads are applied gradually, to give sufficient i time for the strain to fully develop. Variable conditions : stresses vary

### Fatigue Performance Evaluation of Forged Steel versus Ductile Cast Iron Crankshaft: A Comparative Study (EXECUTIVE SUMMARY)

Fatigue Performance Evaluation of Forged Steel versus Ductile Cast Iron Crankshaft: A Comparative Study (EXECUTIVE SUMMARY) Ali Fatemi, Jonathan Williams and Farzin Montazersadgh Professor and Graduate

### The atomic packing factor is defined as the ratio of sphere volume to the total unit cell volume, or APF = V S V C. = 2(sphere volume) = 2 = V C = 4R

3.5 Show that the atomic packing factor for BCC is 0.68. The atomic packing factor is defined as the ratio of sphere volume to the total unit cell volume, or APF = V S V C Since there are two spheres associated

### Investigation of Stress Intensity Factor of Axial Compressor Blade of Helicopter

Investigation of Stress Intensity Factor of Axial Compressor Blade of Helicopter Neelesh V K Mr. Manjunath M V Mr. Devaraj Dept. of Mechanical Engineering Asst prof, Dept. of Mechanical Engineering Asst

### REHABILITATION OF THE FIGUEIRA DA FOZ BRIDGE

REHABILITATION OF THE FIGUEIRA DA FOZ BRIDGE A.Rito Proponte, Lda, Lisbon, Portugal J. Appleton A2P Consult, Lda, Lisbon, Portugal ABSTRACT: The Figueira da Foz Bridge includes a 405 m long cable stayed

### Flaw Size Acceptance Limits for a Stainless Steel Pressure Vessel

Flaw Size Acceptance Limits for a Stainless Steel Pressure Vessel Consuelo Guzman-Leong Lucius Pitkin, Inc. Richland, Washington, U.S.A. Frederic A. Simonen, Ph.D. Lucius Pitkin, Inc. Richland, Washington,

### Comparison of typical 3D printing materials [1]

Comparison of typical 3D printing materials [1] ABS Its strength, flexibility, machinability, and higher temperature resistance make it often a preferred plastic for engineers, and professional applications.

### Description of mechanical properties

ArcelorMittal Europe Flat Products Description of mechanical properties Introduction Mechanical properties are governed by the basic concepts of elasticity, plasticity and toughness. Elasticity is the

### Solved with COMSOL Multiphysics 4.3

Vibrating String Introduction In the following example you compute the natural frequencies of a pre-tensioned string using the 2D Truss interface. This is an example of stress stiffening ; in fact the

### Tensile Testing. Objectives

Laboratory 1 Tensile Testing Objectives Students are required to understand the principle of a uniaxial tensile testing and gain their practices on operating the tensile testing machine. Students are able

### 1. Introduction. 2. Response of Pipelines

1. Introduction Blasting is common in the coal industry to remove rock overburden so that the exposed coal can be mechanically excavated. A portion of the blast energy released is converted to wave energy

### PROPERTIES OF MATERIALS

1 PROPERTIES OF MATERIALS 1.1 PROPERTIES OF MATERIALS Different materials possess different properties in varying degree and therefore behave in different ways under given conditions. These properties

### Multiaxial Fatigue. Professor Darrell Socie. 2008-2014 Darrell Socie, All Rights Reserved

Multiaxial Fatigue Professor Darrell Socie 2008-2014 Darrell Socie, All Rights Reserved Outline Stresses around holes Crack Nucleation Crack Growth MultiaxialFatigue 2008-2014 Darrell Socie, All Rights

### Design strength of optical glass

Design strength of optical glass Keith B. Doyle Sigmadyne, Inc. Rochester, NY Mark A. Kahan Optical Research Associates Westborough, MA ABSTRACT Brittle materials such as glass do not possess a single

### Distinguishing strength from toughness. Understanding fracture toughness.

Lecture notes version 20 Oct 2010 Chapter 8 Fracture and fracture toughness A fractured Liberty Ship 8.1 Introduction and synopsis Distinguishing strength from toughness. Understanding fracture toughness.

### Validation of Cable Bolt Support Design in Weak Rock Using SMART Instruments and Phase 2

Validation of Cable Bolt Support Design in Weak Rock Using SMART Instruments and Phase 2 W.F. Bawden, Chair Lassonde Mineral Engineering Program, U. of Toronto, Canada J.D. Tod, Senior Engineer, Mine Design

### Lecture 14. Chapter 8-1

Lecture 14 Fatigue & Creep in Engineering Materials (Chapter 8) Chapter 8-1 Fatigue Fatigue = failure under applied cyclic stress. specimen compression on top bearing bearing motor counter flex coupling

### Tensile Testing of Steel

C 265 Lab No. 2: Tensile Testing of Steel See web for typical report format including: TITL PAG, ABSTRACT, TABL OF CONTNTS, LIST OF TABL, LIST OF FIGURS 1.0 - INTRODUCTION See General Lab Report Format

### ALLOY 7475 PLATE AND SHEET HIGHEST TOUGHNESS/STRENGTH

ALCOA MILL PRODUCTS ALLOY 7475 PLATE AND SHEET HIGHEST TOUGHNESS/STRENGTH ALLOY 7475 DESCRIPTION Alloy 7475 is a controlled toughness alloy developed by Alcoa for sheet and plate applications that require

### POLITECNICO DI TORINO. Engineering Faculty Master s Degree in Aerospace Engineering. Final Thesis

POLITECNICO DI TORINO Engineering Faculty Master s Degree in Aerospace Engineering Final Thesis DETECTION AND ANALYSIS OF BARELY VISIBLE IMPACT DAMAGE AND ITS PROGRESSION ON A COMPOSITE OVERWRAPPED PRESSURE

### Properties of Materials

CHAPTER 1 Properties of Materials INTRODUCTION Materials are the driving force behind the technological revolutions and are the key ingredients for manufacturing. Materials are everywhere around us, and

### METU DEPARTMENT OF METALLURGICAL AND MATERIALS ENGINEERING

METU DEPARTMENT OF METALLURGICAL AND MATERIALS ENGINEERING Met E 206 MATERIALS LABORATORY EXPERIMENT 1 Prof. Dr. Rıza GÜRBÜZ Res. Assist. Gül ÇEVİK (Room: B-306) INTRODUCTION TENSION TEST Mechanical testing

### MCEN 2024, Spring 2008 The week of Apr 07 HW 9 with Solutions

MCEN 2024, Spring 2008 The week of Apr 07 HW 9 with Solutions The Quiz questions based upon HW9 will open on Thursday, Apr. 11 and close on Wednesday, Apr 17 at 1:30 PM. References to A&J: Chapters 13,

### Master of Simulation Techniques. Lecture No.5. Blanking. Blanking. Fine

Master of Simulation Techniques Lecture No.5 Fine Blanking Prof. Dr.-Ing. F. Klocke Structure of the lecture Blanking Sheared surface and force Wear Blanking processes and blanking tools Errors on sheared

### MODELING THE EFFECT OF TEMPERATURE AND FREQUENCY ON BITUMEN-COATED HELICAL CABLE ELEMENTS

MODELING THE EFFECT OF TEMPERATURE AND FREQUENCY ON BITUMEN-COATED HELICAL CABLE ELEMENTS Bjørn Konradsen 1 Technological Analyses Centre, Hybrid Underwater Cables, Nexans Norway Steinar V. Ouren Material

### Ferrous metal (The sensing distance decreases with non-ferrous metal.) Power supply voltage (operating voltage range)

Description The sensors provide excellent results even with difficult-to-detect objects, e.g. small or thin parts, wires or bright metals. A variety of types cover a wide range of individual requirements

### INFLUENCE OF SHOT PEENING ON CHROMIUM- ELECTROPLATED AISI 4340 STEEL FATIGUE STRENGTH

INFLUENCE OF SHOT PEENING ON CHROMIUM- ELECTROPLATED AISI 4340 STEEL FATIGUE STRENGTH *Voorwald, H. J. C., Silva, M. P., Costa, M. Y. P., a Pigatin, L. W., Marques, B. M. F. Fatigue and Aeronautic Research

### LOAD-CARRYING CAPACITY OF AXIALLY LOADED RODS GLUED-IN PERPENDICULAR TO THE GRAIN

LOAD-CARRYING CAPACITY OF AXIALLY LOADED RODS GLUED-IN PERPENDICULAR TO TE GRAIN Prof. Dr.-Ing..J. Blaß, Dipl.-Ing. B. Laskewitz Universität Karlsruhe (T), Germany Abstract Glued-in rods have been used

### FATIGUE PROPERTIES OF 7175 ALUMINIUM ALLOY HAND FORGINGS. Vladivoj Očenášek

1. -. 11. 1, Plzeň, Czech Republic, EU FATIGUE PROPERTIES OF 717 ALUMINIUM ALLOY HAND FORGINGS Vladivoj Očenášek SVÚM a.s., Podnikatelská 6, 1 11 Praha 9 Běchovice, Czech Republic, ocenasek@svum.cz Abstract

### CHAPTER 6 MECHANICAL PROPERTIES OF METALS PROBLEM SOLUTIONS

CHAPTER 6 MECHANICAL PROPERTIES OF METALS PROBLEM SOLUTIONS Concepts of Stress and Strain 6.1 Using mechanics of materials principles (i.e., equations of mechanical equilibrium applied to a free-body diagram),

### The Mechanical Properties of Glass

The Mechanical Properties of Glass Theoretical strength, practical strength, fatigue, flaws, toughness, chemical processes Glass Engineering 150:312 Professor Richard Lehman Department of Ceramics and

### FATIGUE ANALYSES OF AERONAUTICAL STRUCTURAL DETAILS OF DIFFERENT COMPLEXITY

FATIGUE ANALYSES OF AERONAUTICAL STRUCTURAL DETAILS OF DIFFERENT COMPLEXITY Paulo M S T de Castro, Paulo F P de Matos, Pedro M G P Moreira, Lucas F M da Silva IDMEC and Faculdade de Engenharia, Universidade

### Structural Integrity Analysis

Structural Integrity Analysis 1. STRESS CONCENTRATION Igor Kokcharov 1.1 STRESSES AND CONCENTRATORS 1.1.1 Stress An applied external force F causes inner forces in the carrying structure. Inner forces

### Infrared Study of Heat Dissipation under Fatigue Crack Propagation

Infrared Study of Heat Dissipation under Fatigue Crack Propagation O. Plekhov, M. Bannikov, A. erekhina, A. Fedorova Physical foundation of strength Institute of continuous media mechanics RAS str. Ak.

### Reinforced Concrete Design to BS8110 Structural Design 1 Lesson 5

Lesson 5: Deflection in reinforced concrete beams Content 4.1 Introduction 4. Definitions 4..1 Tension 4.. Compression 4.3 Initial sizing 4.3.1 Worked example 4.4 Reinforcement details 4.5 Anchorage at

### 2. FRACTURE MECHANICS

2. FRACTURE MECHANICS Igor Kokcharov 2.1 DEFECTS Structural materials have inner defects such as cracks, which are extreme stress concentrators. There are technological defects shown in diagrams A and

### Uniaxial Tension and Compression Testing of Materials. Nikita Khlystov Daniel Lizardo Keisuke Matsushita Jennie Zheng

Uniaxial Tension and Compression Testing of Materials Nikita Khlystov Daniel Lizardo Keisuke Matsushita Jennie Zheng 3.032 Lab Report September 25, 2013 I. Introduction Understanding material mechanics

### FATIGUE LIFE OF BOLT SUBJECTED TO FATIGUE LOADING CONDITIONS

20 FATIGUE LIFE OF BOLT SUBJECTED TO FATIGUE LOADING CONDITIONS ABSTRACT K. Din and M. T. H. Ghazali Faculty of Civil Engineering, Universiti Teknologi MARA, Shah Alam, Malaysia E-mail: kdfila@hotmail.com

### Optimum proportions for the design of suspension bridge

Journal of Civil Engineering (IEB), 34 (1) (26) 1-14 Optimum proportions for the design of suspension bridge Tanvir Manzur and Alamgir Habib Department of Civil Engineering Bangladesh University of Engineering

### Time Table. MONDAY (ENS-Cachan) Session 1 : introduction, linear elastic fracture mechanics Session 2 : Exercises. THURSDAY (ENS-Cachan)

Time Table MONDAY (ENS-Cachan) Session 1 : introduction, linear elastic fracture mechanics Session 2 : Exercises TUESDAY (ENS-Cachan) Session 3 : Numerical Practice. Determination of SIF Session 4 : LEFM

### TENSILE TESTING PRACTICAL

TENSILE TESTING PRACTICAL MTK 2B- Science Of Materials Ts epo Mputsoe 215024596 Summary Material have different properties all varying form mechanical to chemical properties. Taking special interest in

### Question 6.5: A steel bar 100 mm (4.0 in.) long and having a square cross section 20 mm

14:440:407 Ch6 Question 6.3: A specimen of aluminum having a rectangular cross section 10 mm 12.7 mm (0.4 in. 0.5 in.) is pulled in tension with 35,500 N (8000 lb f ) force, producing only elastic deformation.

### Tensile fracture analysis of blunt notched PMMA specimens by means of the Strain Energy Density

Engineering Solid Mechanics 3 (2015) 35-42 Contents lists available at GrowingScience Engineering Solid Mechanics homepage: www.growingscience.com/esm Tensile fracture analysis of blunt notched PMMA specimens

### Numerical Analysis of Independent Wire Strand Core (IWSC) Wire Rope

Numerical Analysis of Independent Wire Strand Core (IWSC) Wire Rope Rakesh Sidharthan 1 Gnanavel B K 2 Assistant professor Mechanical, Department Professor, Mechanical Department, Gojan engineering college,

### WELD - STATIC AND FATIGUE STRENGTH -III

32 WELD - STATIC AND FATIGUE STRENGTH -III 1.0 INTRODUCTION A component or a structure, which can withstand a single application of load, may fracture if the same load is applied a large number of times.

### FEM analysis of the forming process of automotive suspension springs

FEM analysis of the forming process of automotive suspension springs Berti G. and Monti M. University of Padua, DTG, Stradella San Nicola 3, I-36100 Vicenza (Italy) guido.berti@unipd.it, manuel.monti@unipd.it.

### Mechanical & Non-Destructive Testing

Training Objective After watching the program and reviewing this printed material, the viewer will gain an understanding and become familiar with the various methods, equipment, and applications of mechanical

### Dentistry Fatigue test for endosseous dental implants. Report No.: 1 ASTRA System Ti Design

Dentistry Fatigue test for endosseous dental implants Report No.: 1 ASTRA System Ti Design Client: NT - Trading Time of execution: Mai 2011 Subject of work: - - S - 24285 Abutment Ti DesignTM - RESULTS

### Modelling of fatigue crack growth in Inconel 718 under hold time conditions - application to a flight spectrum

Modelling of fatigue crack growth in Inconel 718 under hold time conditions - application to a flight spectrum Erik Lundström, Kjell Simonsson, Tomas Månsson and David Gustafsson Linköping University Post

### Hip Replacement Failure Analysis and Design Improvement Techniques

Hip Replacement Failure Analysis and Design Improvement Techniques Kevin W. Jansen Ohio Northern University Ada, OH, 45810 Email: k-jansen@onu.edu ABSTRACT Hip replacements have been utilized widely to

### Ultrasonic Technique and Device for Residual Stress Measurement

Ultrasonic Technique and Device for Residual Stress Measurement Y. Kudryavtsev, J. Kleiman Integrity Testing Laboratory Inc. 80 Esna Park Drive, Units 7-9, Markham, Ontario, L3R 2R7 Canada ykudryavtsev@itlinc.com

### Effect of Heat Treatment Process on the Fatigue Behavior of AISI 1060 Steel

International International Journal of ISSI, Journal Vol. of 12 ISSI, (2015), Vol.10 No.1, (2013), pp. 28-32 No.1 Effect of Heat Treatment Process on the Fatigue Behavior of AISI 1060 Steel M. Mehdinia

### FRETTING FATIGUE UNDER VARYING LOADING BELOW THE FRETTING FATIGUE LIMIT

FRETTING FATIGUE UNDER VARYING LOADING BELOW THE FRETTING FATIGUE LIMIT Yoshiyuki KONDO 1, Chu SAKAE 1, Masanobu KUBOTA 1 and Hiroki KITAHARA 2 1 Kyushu University, Faculty of Engineering, 6-10-1, Hakozaki,

### Mechanical Properties

Mechanical Properties Elastic deformation Plastic deformation Fracture Plastic Instability and the Ultimate Tensile Strength s u P s s y For a typical ductile metal: I. Elastic deformation II. Stable plastic

### Capacitive Proximity Sensor

Capacitive Proximity Sensor X Threaded Cylindrical Capacitive Proximity Sensor Detects almost any kind of metallic and nonmetallic objects, including glass, lumber, water, oil, and plastic. Three choices

### Measuring the Condition of Prestressed Concrete Cylinder Pipe

Measuring the Condition of Prestressed Concrete Cylinder Pipe John Marshall, P.E.I, I J.W. Marshall and Associates, and Paul S. Fisk, President NDT Corporation Introduction Prestressed Concrete Cylinder

### Punching shear behavior of steel-concrete composite decks with different shear connectors

Punching shear behavior of steel-concrete composite decks with different shear connectors *Xiao-Qing Xu 1) and Yu-Qing Liu 2) 1), 2) Department of Bridge Engineering, Tongji University, Shanghai 200092,

### Numerical modelling of shear connection between concrete slab and sheeting deck

7th fib International PhD Symposium in Civil Engineering 2008 September 10-13, Universität Stuttgart, Germany Numerical modelling of shear connection between concrete slab and sheeting deck Noémi Seres

### TENSIONMETER ** code 183_LNRSTW **

Electronic tension meter for applications in textile and wire industry. 9 Tension ranges from 0.1-200 cn to 5-50 dan. Versatile instruments usable for applications in textile industry: e. g. 50 up to max.

### Fatigue Resistance of High Strength Bolts with Large Diameters

1 Fatigue Resistance of High Strength Bolts with Large Diameters Prof. Peter Schaumann; Dipl.-Ing. Frithjof Marten Leibniz Universitaet Hannover Institute for Steel Construction Hannover, Germany schaumann@stahl.uni-hannover.de;

### The Bending Strength of Pasta

The Bending Strength of Pasta 1.105 Lab #1 Louis L. Bucciarelli 9 September, 2003 Lab Partners: [Name1] [Name2] Data File: Tgroup3.txt On the cover page, include your name, the names of your lab partners,

### Yield Criteria for Ductile Materials and Fracture Mechanics of Brittle Materials. τ xy 2σ y. σ x 3. τ yz 2σ z 3. ) 2 + ( σ 3. σ 3

Yield Criteria for Ductile Materials and Fracture Mechanics of Brittle Materials Brittle materials are materials that display Hookean behavior (linear relationship between stress and strain) and which

### Bolting Galvanized Steel

Bolting Galvanized Steel This chapter gives information on the characteristics, advantages and economics of bolted galvanized structures and zinc coated fasteners, and offers comment on bolting procedures

### CHARACTERISATION OF A RESONANT BENDING FATIGUE TEST SETUP FOR PIPES

CHARACTERISATION OF A RESONANT BENDING FATIGUE TEST SETUP FOR PIPES J. Claeys 1, J. Van Wittenberghe 2, P. De Baets 2 and W. De Waele 2 2 1 Ghent University, Belgium Ghent University, laboratory Soete,

### Operating Temperature Range: -30 to +85ç (Note 1) Operating Humidity Range: 40 to 80%

All non- products have been discontinued, or will be discontinued soon. Please check the products status on the Hirose website search at www.hirose-connectors.com, or contact your Hirose sales representative.

### Topology Optimization of Engine Mount Brackets Dr. Dirk Sprengel Ford Werke GmbH

Topology Optimization of Engine Mount Brackets Dr. Dirk Sprengel Ford Werke GmbH Dr. D. Sprengel 6/2007 Topology Optimization of EMS Bracket 1 ( 21 ) EMS Bracket Funktion EMS: Engine Mount System Link

### EDEXCEL NATIONAL CERTIFICATE/DIPLOMA MECHANICAL PRINCIPLES OUTCOME 2 ENGINEERING COMPONENTS TUTORIAL 1 STRUCTURAL MEMBERS

ENGINEERING COMPONENTS EDEXCEL NATIONAL CERTIFICATE/DIPLOMA MECHANICAL PRINCIPLES OUTCOME ENGINEERING COMPONENTS TUTORIAL 1 STRUCTURAL MEMBERS Structural members: struts and ties; direct stress and strain,

### Tutorial: Calculation of paired angular contact bearings

Tutorial: Calculation of paired angular contact bearings A pair of angular contact ball bearings mounted back-to-back should be calculated for a load case radial load only, and a second load case tilting

### Modular Plug Connectors compliant to Cat.6 A Standard

Modular Plug Connectors compliant to Cat.6 A Standard TM3P Series Features. Support High-Speed LAN transmission Improved performance by two row contact arrangement. Conforms to Cat.6 A requirements of

### FRETTING FATIGUE CRACKlNG OF A 936 MW TURBO- GENERATOR ROTOR FAILURE ANALYSIS AND REFURBISHMENT

FRETTING FATIGUE CRACKlNG OF A 936 MW TURBO- GENERATOR ROTOR FAILURE ANALYSIS AND REFURBISHMENT Dr. K. Schöllhorn 1 Dr. G. Ebi 2 K. Steigleder 1 1 ABB Power Generation Ltd Switzerland 2 SENSOPLAN GmbH